complexesNATALIA V. KAMANINA1, JAN OWSIK2*, BEATA RUSEK3
1Vavilov State Optical Institute, 12 Birzhevaya Line St., St.-Petersburg 199034, Russia 2Military University of Technology, 2 Kaliskiego St., 00-908 Warsaw, Poland 3WELDI S.C., 1 Pszczyńska St., 43-175 Wyry, Poland
*Corresponding author: email@example.com; firstname.lastname@example.org
We have observed the piezoelectric and elastooptic effects for the 2-cyclooctylamino-5-nitropyr-idine complex, chromophore doped by an inter-molecular acceptor – fullerene C70. The discovered features may be used for optically operated piezoelectric triggers, modulators and deflectors. The observed effects are caused by the effective interaction of external light with the polarizable chromophore. As a pumping laser beam we have used both a nanosecond fundamental 1064 nm laser wavelength as well as its second harmonic generation at 532 nm. A principal role in the ob-served effects play photoinduced anharmonic phonons, effectively contributing to the output effect. Keywords: nonlinear media, piezooptical effect, 2-cyclooctylamino-5-nitropyridine (COANP), fullerene,
Recent developments in laser technique and optically operated piezoelectric sources favor an interest in extensive research and designing of new nonlinear optical, piezooptical and piezoelectric materials possessing embedded effective nanochromo-phores. The latter are especially important for production of laser operated devices like triggers, modulators, memory and deflector devices [1–7]. These technical re-quirements stimulated an effective search for optical materials, with properties which can effectively change their optical and piezooptical coefficients. Among these mate-rials, the systems based on 2-cyclooctylamino-5-nitropyridine (COANP) (see Fig. 1) play a unique role due to their highly charge transferred delocalized π-conjugated electron states. It is necessary to emphasize that such chromophores have just been partially studied, what was reported in Refs. [8–13].
COANP chromophore is a promising molecule with an effective intra-molecular charge transfer process between the NH– (donor) and NO2– (acceptor). This
intra-molec-ular charge transfer can be modified using molecintra-molec-ular materials engineering. Their electron affinity energies for intra-molecular acceptor fragments of COANP are varied between 0.4–0.54 eV. For example, the electron affinity energy of C60 and C70 is equal to about 2.65 eV. Thus, the inter-molecular acceptor fragment electron affinity energy is at least five times higher. Therefore, embedded chromophores are stronger sensitiz-ers and they determine the acceptor fragments of an intra-molecular molecule. In this case, the intra-molecular electrostatic field gradient leads to an enhanced ground state dipole moment. So the increase in local volume polarizability stimulates the increase in dipole polarizability as well as the increase in charge carrier mobility.
In this paper we present the studies of laser induced piezoelectricity and piezooptics of the COANP system (see Fig. 1) doped with fullerene C70. It may be recommended for use as a promising material for photoinduced acoustooptical modulators operated by external light.
In our experiments, the fullerene-doped COANP films possessing thickness equal to about 3–4μm thick were prepared by spin-coating of the solution in 1,1,2,2,-tetra-chloroetane on a glass substrate. A small amount of non-photosensitive polyimide structure has been used as a plasticizer in order to form the homogenous solid film. The fullerene concentration was varied within 0.5–5 wt%. Absorption spectra of the investigated systems were measured by a Perkin Elmer Lambda 9 spectrometer in the 200–3000 nm region with spectral resolution of about 0.5 nm.
The photoinduced piezoelectric and elastic changes were excited by Nd:YAG laser operating at 1064 nm in 15 ns regime with frequency repetition up to 1.2 kHz. The pulse energy of the 1064 nm photoinducing laser was varied within the 40–70 mJ and the pulse energy of the frequency doubled using BiB3O6 single crystal was equal to 20–30 mJ. Its diameter was fixed at 3–4 mm and the Gaussian-like contour was
Fig. 1. COANP molecule. NO2
used. The incident angle of the photoinducing laser beam was varied within 22–24° to achieve the maximal output response.
The probing of the piezooptical effect was measured by a cw He-Ne laser with the powered density 3 mW, to exclude any overheating. The traditional Senarmont meth-od used for analogous studies of other polymer composites was applied (see Fig. 2). Usually the mechanical field was applied by an external piezoelectric transducer which formed the mechanical field at a frequency of about 1 MHz. The same field was used for the measurement of the piezoelectric coefficient. The set-up allows for registration of the changes in the birefringence with a precision up to 10–6 and of the piezoelectric
coefficient with a precision up to 0.1 pm/V. The method is partially similar to Ref. . The laser treatment was done simultaneously with the 1μs CO2 laser treatment.
The observed effect achieved its maximum after 4–6 min of the photoinduced treat-ment and was controlled by the saturation of a CO2 laser beam.
3. Results and discussion
Absorption spectra of the system studied are shown in Fig. 3. The absorption spectrum of COANP–polyimide–fullerene composite shows substantially different spectral fea-tures than the spectra of COANP–polyimide or polyimide–C70 systems. There are two additional absorption peaks – at 490 nm and 810–820 nm. In the present paper we ex-plain these peculiarities with inter-molecular charge transfer features and support them via analytic calculations, mass-spectrometry and nonlinear optical experiments [11–13]. It should be emphasized that for all investigated COANP systems, the nonlinear charac-teristics lie within the range: n2= 10–10–10–9cm2W–1 and χ(3) = 10–10–10–9cm3erg–1.
In comparison, for quartz, which is a classical material traditionally used for nonlinear optics, the values of n2 and χ(3) are (2.5–3)×10–16cm–2W–1 and 10–14cm3erg–1 (esu),
respectively. Thus, the systems studied reveal increased nonlinear optical parameters via photorefractive estimation.
Fig. 2. Measurement set-up for photoinduced piezoelectrics and piezooptics. PMT – piezomodulated transducer, PD – photodetector.
The photoinduced piezoelectrics for the d32 tensor component was higher for the 532 nm wavelength and less for the 1064 nm nanosecond laser pulses (see Fig. 4). This indicates on the substantial influence of the absorption edge in the observed photoinduced dependences.
The performed photoinduced piezooptical experiments have shown that the maximal photoinduced piezooptical effect was achieved for fullerene-doped COANP structure. However, these effects are maximal for the diagonal tensor coefficients (see Fig. 5). For the remaining three structures this effect was at least one order less. Moreover, the illumination by 532 nm gives the photoinduced changes at least 3 times higher (see Fig. 5) which correlates with the photoinduced piezoelectricity. It is interesting that
0.5 0.0 400 600 800 1000 1200 1400 1 2 3 4
Optical density [a. u.]
Fig. 3. Absorption spectra: 1 – fullerene-doped COANP–polyimide structure, 2 – pure polyimide, 3 – C70-doped polyimide, and 4 – fullerene-free COANP–polyimide.
0.30 0.15 0.00 0 100 200 300 532 nm 1064 nm deff [pm /V ] I [MW/cm2]
Fig. 4. Photoinduced piezoelectric efficient d23 coefficient at different photoinducing wavelengths for fullerene-doped COANP–polyimide structure.
the maximal effect was observed at power density equal to about 260 MW/cm2. At
higher intensities there occurs some material’s photodestruction.
The relaxation times of the effect do not exceed 6 minutes and the process is completely reproducible during many cycles. The existence of the effect for fuller-ene-doped COANP–polyimide structure may be caused by the existence of an effec-tive charge transfer which is demonstrated by the absorption spectra presented in Fig. 3 together with the specific contribution of the electron–phonon interaction. It is well-known that the third-order nonlinear piezooptical effects as well as other third-order nonlinear optical susceptibilities are very sensitive to the contribution of the electron–phonon interactions [14, 15]. Additionally, very crucial are interfaces separating the polymers and the embedded chromophores [16, 17]. It is caused by some flattering of the delocalized states due to the low-dimensional periodicity  and electron–phonon anharmonicities  together with the influence of the multi-photon processes .
The photoinduced piezooptical effect was discovered under the influence of the optical treatment by the 1064 nm nanosecond and its second harmonic generation. Moreover, the illumination by 532 nm shows that the photoinduced changes are at least 3 times higher. It is interesting that the maximal effect was observed at power density equal to about 260 MW/cm2. At higher processes, the process is less due to the multi-photon
excitations. The photoinduced piezoelectrics for the d32 tensor component was higher for the 532 nm wavelength and less for the 1064 nm nanosecond laser pulses what indicates on the substantial influence of the absorption edge in the observed photoinduced dependences. The observed effect is a consequence of the substantial
0 100 200 300
Fig. 5. Photoinduced piezooptical effect for diagonal tensor coefficient at different photoinducing wavelengths for fullerene-doped COANP–polyimide structure.
contribution of the photoexcited phonon subsystem. The comparison with the similar chromophore confirms a principal role of the π-conjugated charge transfer due to the interaction with an electron–phonon subsystem.
 WANG Y., HERRON N., CASPER J., Bucky ball and quantum dot doped polymers: a new class of
optoelectronic materials, Materials Science and Engineering B 19(1–2), 1993, pp. 61–66.
 ROBERTSON J., Realistic applications of CNTs, Materials Today 7(10), 2004, pp. 46–52.
 WEI LEEAND HSU-CHIH CHEN, Diffraction efficiency of a holographic grating in a liquid-crystal cell
composed of asymmetrically patterned electrodes, Nanotechnology 14(9), 2003, pp. 987–990.
 BUCHNEV O., DYADYUSHA A., KACZMAREK M., RESHETNYAK V., REZNIKOV YU., Enhanced two-beam
coupling in colloids of ferroelectric nanoparticles in liquid crystals, Journal of the Optical Society
of America B 24(7), 2007, pp. 1512–1516.
 GRISHINA A.D., LICEA-JIMENE L., PERESHIVKO L.YA., KRIVENKO T.V., SAVEL’EV V.V., RYCHWALSKI R.W., VANNIKOV A.V., Infrared photorefractive composites based on
polyvinylcarba-zole and carbon nanotubes, High Energy Chemistry 40(5), 2006, pp. 341–347.
 KAMANINA N.V., EMANDI A., KAJZAR F., ATTIAS A.-J., Laser-induced change in the refractive index
in the systems based on nanostructured polyimide: comparative study with other photosensitive structures, Molecular Crystals and Liquid Crystals 486(1), 2008, pp. 1–11.
 KAMANINA N.V., SEROV S.V, SHURPO N.A., LIKHOMANOVA S.V., TIMONIN D.N., KUZHAKOV P.V., ROZHKOVA N.N., KITYK I.V, PLUCINSKI K.J., USKOVIC D.P., Polyimide-fullerene nanostructured
materials for nonlinear optics and solar energy applications, Journal of Materials Science: Materials
in Electronics 23(8), 2012, pp. 1538–1542.
 JIN YAN, MEIZI JIAO, LINGHUI RAO, SHIN-TSON WU, Direct measurement of electric-field-induced
birefringence in a polymer-stabilized blue-phase liquid crystal composite, Optics Express 18(11),
2010, pp. 11450–11455.
 SUTTR K., HULLIGER J., GUNTER P., Photorefractive effects observed in the organic crystal
2-cyclo-octylamino-5-nitropyridine doped with 7,7,8,8-tetracyanoquinodimethane, Solid State
Communi-cations 74(8), 1990, pp. 867–870.
 LEYDERMAN A., CUI Y., Electro-optical characterization of a 2-cyclo-octylamino-5-nitropyridine
thin organic crystal film, Optics Letters 23(12), 1998, pp. 909–911.
 KAMANINA N.V., BARRIENTOS A., LEYDERMAN A., CUI Y., VIKHNIN V., VLASSE M., Effect of fullerene
doping on the absorption edge shift in COANP, Molecular Materials 13(1–4), 2000, pp. 275–280.
 KAMANINA N.V., Peculiarities of optical limiting effect in π-conjugated organic systems based
on 2-cyclooctylamino-5-nitropyridine doped with C70, Journal of Optics A: Pure and Applied Optics 3(5), 2001, pp. 321–325.
 KAMANINA N.V., PLEKHANOV A.I., Mechanisms of optical limiting in fullerene-doped π-conjugated
organic structures demonstrated with polyimide and COANP molecules, Optics and Spectroscopy 93(3), 2002, pp. 408–415.
 KITYK I.V., KASPERCZYK J., SAHRAOUI B., YASINSKII M.F., HOLAN B., Low temperature anomalies in
polivinyl alcohol photopolymers, Polymer 38(19), 1997, pp. 4803–4806.
 SAHRAOUI B., DERKOWSKA B., KRYZA A., KITYK I.V., The IR photoinduced changes in the Y–Ba–
–Cu–O thin films, Optica Applicata 31(2), 2001, pp. 445–451.
 KITYK I. V., MAKOWSKA-JANUSIK M., GONDEK E., KRZEMINSKA L., DANEL A., PLUCINSKI K.J., BENET S., SAHRAOUI B., Optical poling of oligoether acrylate photopolymers doped by stilbene-benzoate
derivative chromophores, Journal of Physics: Condensed Matter 16(3), 2004, pp. 231–239.
 KOSCIEN E., SANETRA J., GONDEK E., JAROSZ B., KITYK I.V., EBOTHE J., KITYK A.V., Optical poling
of several halogen derivatives of pyrazoloquinoline, Optics Communications 242(4–6), 2004,
Received October 5, 2012 in revised form November 21, 2012